| ||Format||Pages||Price|| |
|14||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||14||$52.00||  ADD TO CART|
Significance and Use
5.1 Soil placed as engineering fill (embankments, foundation pads, road bases) is compacted to a dense state to obtain satisfactory engineering properties such as shear strength, compressibility, or permeability. In addition, foundation soils are often compacted to improve their engineering properties. Laboratory compaction tests provide the basis for determining the percent compaction and molding water content needed to achieve the required engineering properties, and for controlling construction to assure that the required compaction and water contents are achieved.
Note 3: The degree of soil compaction required to achieve the desired engineering properties is often specified as a percentage of the modified maximum dry unit weight as determined using this test method. If the required degree of compaction is substantially less than the modified maximum dry unit weight using this test method, it may be practicable for testing to be performed using Test Method (. Use of ) , on the other hand, allows compaction using less effort and generally at a higher optimum moisture content. The compacted soil may be less brittle, more flexible, more permeable, and less subject to effects of swelling and shrinking. In many applications, building or construction codes may direct which test method, or this one, should be used when specifying the comparison of laboratory test results to the degree of compaction of the in-place soil in the field. and to specify the degree of compaction as a percentage of the standard maximum dry unit weight. Since more energy is applied for compaction using this test method, the soil particles are more closely packed than when is used. The general overall result is a higher maximum dry unit weight, lower optimum moisture content, greater shear strength, greater stiffness, lower compressibility, lower air voids, and decreased permeability. However, for highly compacted fine-grained soils, absorption of water may result in swelling, with reduced shear strength and increased compressibility, reducing the benefits of the increased effort used for compaction
5.2 During design of an engineered fill, testing performed to determine shear, consolidation, permeability, or other properties requires test specimens to be prepared by compacting the soil at a prescribed molding water content to obtain a predetermined unit weight. It is common practice to first determine the optimum water content (wopt) and maximum dry unit weight (γdmax) by means of a compaction test. Test specimens are compacted at a selected molding water content (w), either wet or dry of optimum (wopt) or at optimum (wopt), and at a selected dry unit weight related to a percentage of maximum dry unit weight (γdmax). The selection of molding water content (w), either wet or dry of optimum (wopt) or at optimum (wopt) and the dry unit weight (γdmax) may be based on past experience, or a range of values may be investigated to determine the necessary percent of compaction.
5.3 Experience indicates that the methods outlined in or the construction control aspects discussed in are extremely difficult to implement or yield erroneous results when dealing with some soils. The following subsections describe typical problem soils, the problems encountered when dealing with such soils and possible solutions for these problems.
5.3.1 Oversize Fraction—Soils containing more than 30 % oversize fraction (material retained on the 3/4-in. (19-mm) sieve) are a problem. For such soils, there is no ASTM test method to control their compaction and very few laboratories are equipped to determine the laboratory maximum unit weight (density) of such soils (USDI Bureau of Reclamation, Denver, CO and U.S. Army Corps of Engineers, Vicksburg, MS). Although Test Methods and determine the “field” dry unit weight of such soils, they are difficult and expensive to perform.
188.8.131.52 One method to design and control the compaction of such soils is to use a test fill to determine the required degree of compaction and the method to obtain that compaction. Then use a method specification to control the compaction. Components of a method specification typically contain the type and size of compaction equipment to be used, the lift thickness, acceptable range of molding water content, and number of passes.
Note 4: Success in executing the compaction control of an earthwork project, especially when a method specification is used, is highly dependent upon the quality and experience of the contractor and inspector.
184.108.40.206 Another method is to apply the use of density correction factors developed by the USDI Bureau of Reclamation ( and U.S. Corps of Engineers , )(. These correction factors may be applied for soils containing up to about 50 to 70 % oversize fraction. Both agencies use a different term for these density correction factors. The USDI Bureau of Reclamation uses )D ratio (or D – VALUE), while the U.S. Corps of Engineers uses Density Interference Coefficient (Ic).
220.127.116.11 The use of the replacement technique (Test Method –78, Method D), in which the oversize fraction is replaced with a finer fraction, is inappropriate to determine the maximum dry unit weight, γdmax, of soils containing oversize fractions (. )
5.3.2 Degradation—Soils containing particles that degrade during compaction are a problem, especially when more degradation occurs during laboratory compaction than field compaction, the typical case. Degradation typically occurs during the compaction of a granular-residual soil or aggregate. When degradation occurs, the maximum dry-unit weight increases ( so that the resulting laboratory maximum value is not representative of field conditions. Often, in these cases, the maximum dry unit weight is impossible to achieve in the field. )
18.104.22.168 Again for soils subject to degradation, the use of test fills and method specifications may help. Use of replacement techniques is not correct.
5.3.3 Gap Graded—Gap-graded soils (soils containing many large particles with limited small particles) are a problem because the compacted soil will have larger voids than usual. To handle these large voids, standard test methods (laboratory or field) typically have to be modified using engineering judgement.
Note 5: The quality of the result produced by this standard is dependent on the competence of the personnel performing it, and the suitability of the equipment and facilities used. Agencies that meet the criteria of Practice are generally considered capable of competent and objective testing/sampling/inspection/etc. Users of this standard are cautioned that compliance with Practice does not in itself assure reliable results. Reliable results depend on many factors; Practice provides a means of evaluating some of those factors.
1.1 These test methods cover laboratory compaction methods used to determine the relationship between molding water content and dry unit weight of soils (compaction curve) compacted in a 4- or 6-in. (101.6- or 152.4-mm) diameter mold with a 10.00-lbf. (44.48-N) rammer dropped from a height of 18.00 in. (457.2 mm) producing a compactive effort of 56 000 ft-lbf/ft3 (2700 kN-m/m3).
Note 1: The equipment and procedures are the same as proposed by the U.S. Corps of Engineers in 1945. The modified effort test (see ) is sometimes referred to as the Modified Proctor Compaction Test.
1.1.1 Soils and soil-aggregate mixtures are to be regarded as natural occurring fine- or coarse-grained soils, or composites or mixtures of natural soils, or mixtures of natural and processed soils or aggregates such as gravel or crushed rock. Hereafter referred to as either soil or material.
1.2 These test methods apply only to soils (materials) that have 30 % or less by mass of their particles retained on the 3/4-in. (19.0-mm) sieve and have not been previously compacted in the laboratory; that is, do not reuse compacted soil.
1.2.1 For relationships between unit weights and molding water contents of soils with 30 % or less by weight of material retained on the 3/4-in. (19.0-mm) sieve to unit weights and molding water contents of the fraction passing the 3/4-in. (19.0-mm) sieve, see Practice .
1.3 Three alternative methods are provided. The method used shall be as indicated in the specification for the material being tested. If no method is specified, the choice should be based on the material gradation.
1.3.1 Method A:
22.214.171.124 Mold—4-in. (101.6-mm) diameter.
126.96.36.199 Material—Passing No. 4 (4.75-mm) sieve.
188.8.131.52 Blows per layer—25.
184.108.40.206 Usage—May be used if 25 % or less by mass of the material is retained on the No. 4 (4.75-mm) sieve. However, if 5 to 25 % by mass of the material is retained on the No. 4 (4.75-mm) sieve, Method A can be used but oversize corrections will be required (See ) and there are no advantages to using Method A in this case.
220.127.116.11 Other Use—If this gradation requirement cannot be met, then Methods B or C may be used.
1.3.2 Method B:
18.104.22.168 Mold—4-in. (101.6-mm) diameter.
22.214.171.124 Material—Passing 3/8-in. (9.5-mm) sieve.
126.96.36.199 Blows per layer—25.
188.8.131.52 Usage—May be used if 25 % or less by mass of the material is retained on the 3/8-in. (9.5-mm) sieve. However, if 5 to 25 % of the material is retained on the 3/8-in. (9.5-mm) sieve, Method B can be used but oversize corrections will be required (See ). In this case, the only advantages to using Method B rather than Method C are that a smaller amount of sample is needed and the smaller mold is easier to use.
184.108.40.206 Other Usage—If this gradation requirement cannot be met, then Method C may be used.
1.3.3 Method C:
220.127.116.11 Mold—6-in. (152.4-mm) diameter.
18.104.22.168 Material—Passing 3/4-in. (19.0-mm) sieve.
22.214.171.124 Blows per layer—56.
126.96.36.199 Usage—May be used if 30 % or less (see ) by mass of the material is retained on the 3/4-in. (19.0-mm) sieve.
1.3.4 The 6-in. (152.4-mm) diameter mold shall not be used with Method A or B.
Note 2: Results have been found to vary slightly when a material is tested at the same compactive effort in different size molds, with the smaller mold size typically yielding larger values of unit weight and density (. )
1.4 If the test specimen contains more than 5 % by mass of oversize fraction (coarse fraction) and the material will not be included in the test, corrections must be made to the unit weight and molding water content of the test specimen or to the appropriate field in-place unit weight (or density) test specimen using Practice .
1.5 This test method will generally produce a well-defined maximum dry unit weight for non-free draining soils. If this test method is used for free-draining soils the maximum unit weight may not be well defined, and can be less than obtained using Test Methods .
1.6 All observed and calculated values shall conform to the guidelines for significant digits and rounding established in Practice , unless superseded by these test methods.
1.6.1 For purposes of comparing measured or calculated value(s) with specified limits, the measured or calculated value(s) shall be rounded to the nearest decimal or significant digits in the specified limits.
1.6.2 The procedures used to specify how data are collected/recorded or calculated in this standard are regarded as the industry standard. In addition, they are representative of the significant digits that generally should be retained. The procedures used do not consider material variation, purpose for obtaining the data, special purpose studies, or any considerations for the user’s objectives; it is common practice to increase or reduce significant digits of reported data to be commensurate with these considerations. It is beyond the scope of these test methods to consider significant digits used in analytical methods for engineering design.
1.7 The values in inch-pound units are to be regarded as the standard. The values stated in SI units are provided for information only, except for units of mass. The units for mass are given in SI units only, g or kg.
1.7.1 It is common practice in the engineering profession to concurrently use pounds to represent both a unit of mass (lbm) and a force (lbf). This implicitly combines two separate systems of units; that is, the absolute system and the gravitational system. It is scientifically undesirable to combine the use of two separate sets of inch-pound units within a single standard. These test methods have been written using the gravitational system of units when dealing with the inch-pound system. In this system, the pound (lbf) represents a unit of force (weight). However, the use of balances or scales recording pounds of mass (lbm) or the recording of density in lbm/ft3 shall not be regarded as a nonconformance with this standard.
1.8 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
1.9 Warning—Mercury has been designated by EPA and many state agencies as a hazardous material that can cause central nervous system, kidney, and liver damage. Mercury, or its vapor, may be hazardous to health and corrosive to materials. Caution should be taken when handling mercury and mercury containing products. See the applicable product Material Safety Data Sheet (MSDS) for details and EPA’s website (http://www.epa.gov/mercury/faq.htm) for additional information. Users should be aware that selling mercury or mercury containing products or both into your state may be prohibited by state law.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C127 Test Method for Relative Density (Specific Gravity) and Absorption of Coarse Aggregate
C136 Test Method for Sieve Analysis of Fine and Coarse Aggregates
C670 Practice for Preparing Precision and Bias Statements for Test Methods for Construction Materials
D653 Terminology Relating to Soil, Rock, and Contained Fluids
D698 Test Methods for Laboratory Compaction Characteristics of Soil Using Standard Effort (12 400 ft-lbf/ft3 (600 kN-m/m3))
D854 Test Methods for Specific Gravity of Soil Solids by Water Pycnometer
D2168 Practices for Calibration of Laboratory Mechanical-Rammer Soil Compactors
D2216 Test Methods for Laboratory Determination of Water (Moisture) Content of Soil and Rock by Mass
D2487 Practice for Classification of Soils for Engineering Purposes (Unified Soil Classification System)
D2488 Practice for Description and Identification of Soils (Visual-Manual Procedure)
D3740 Practice for Minimum Requirements for Agencies Engaged in Testing and/or Inspection of Soil and Rock as Used in Engineering Design and Construction
D4220 Practices for Preserving and Transporting Soil Samples
D4253 Test Methods for Maximum Index Density and Unit Weight of Soils Using a Vibratory Table
D4718 Practice for Correction of Unit Weight and Water Content for Soils Containing Oversize Particles
D4753 Guide for Evaluating, Selecting, and Specifying Balances and Standard Masses for Use in Soil, Rock, and Construction Materials Testing
D4914 Test Methods for Density and Unit Weight of Soil and Rock in Place by the Sand Replacement Method in a Test Pit
D5030 Test Method for Density of Soil and Rock in Place by the Water Replacement Method in a Test Pit
D6026 Practice for Using Significant Digits in Geotechnical Data
D6913 Test Methods for Particle-Size Distribution (Gradation) of Soils Using Sieve Analysis
E11 Specification for Woven Wire Test Sieve Cloth and Test Sieves
E319 Practice for the Evaluation of Single-Pan Mechanical Balances
ICS Number Code 93.020 (Earth works. Excavations. Foundation construction. Underground works)
UNSPSC Code 11111501(Soil)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D1557-12e1, Standard Test Methods for Laboratory Compaction Characteristics of Soil Using Modified Effort (56,000 ft-lbf/ft3 (2,700 kN-m/m3)), ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top